Martensite in Steels


 Julie Nelson
 2 years ago
 Views:
Transcription
1 Materials Science & Metallurgy H. K. D. H. Bhadeshia Martensite in Steels The name martensite is after the German scientist Martens. It was used originally to describe the hard microconstituent found in quenched steels. Martensite remains of the greatest technological importance in steels where it can confer an outstanding combination of strength (> 3500 MPa) and toughness (> 200 MPa m 1 2 ). Many materials other than steel are now known to exhibit the same type of solidstate phase transformation, known as a martensitic transformation, frequently also called a shear or displacive transformation. Martensite occurs in, for example, nonferrous alloys, pure metals, ceramics, minerals, inorganic compounds, solidified gases and polymers (Table 1). We shall review first the experimental facts about martensite and then proceed to explain them. Composition M S / K Hardness HV ZrO Fe 31Ni 0.23C wt% Fe 34Ni 0.22C wt% < Fe 3Mn 2Si 0.4C wt% Cu 15Al Ar 40N 2 30 Table 1: The temperature M S at which martensite first forms on cooling, and the approximate Vickers hardness of the resulting martensite for a number of materials. Diffusionless Character Martensitic transformations are diffusionless, but what evidence is there to support this? Martensite can form at very low temperatures, where diffusion, even of interstitial atoms, is not conceivable over the time period of the experiment. Table 1 gives values of the highest temperature at which martensite forms in a variety of materials; this temperature is known as the martensite start, or M S temperature. It is obvious that although martensite can form 1
2 at low temperatures, it need not do so. Therefore, a low transformation temperature is not sufficient evidence for diffusionless transformation. Martensite plates can grow at speeds which approach that of sound in the metal. In steel this can be as high as 1100 m s 1, which compares with the fastest recorded solidification front velocity of about 80 m s 1 in pure nickel. Such large speeds are inconsistent with diffusion during transformation. Note that martensite need not grow so rapidly. For example, in shape memory alloys or in single interface transformations, the interface velocity is small enough to observe. The chemical composition of martensite can be measured and shown to be identical to that of the parent austenite. The totality of these observations demonstrate convincingly that martensitic transformations are diffusionless. The Habit Plane This is the interface plane between austenite and martensite as measured on a macroscopic scale (Fig. 1), for example by using one or two surface crystallographic trace analysis on metallographic samples. For unconstrained transformations this interface plane is flat, but strain energy minimisation introduces some curvature when the transformation is constrained by its surroundings. Nevertheless, the macroscopic habit plane is identical for both cases, as illustrated in Figure 1. Figure 1: An illustration of the habit plane between austenite (γ) and martensite (α ) 2
3 Steels of vastly different chemical composition can have martensite with the same habit plane (Table 2), and indeed, other identical crystallographic characteristics. Composition /wt.% Low alloy steels, Fe 28Ni Plate martensite in Fe 1.8C Fe 30Ni 0.3C Fe 8Cr 1C ɛ martensite in 18/8 stainless steel Approximate habit plane indices {1 1 1} γ {2 9 5} γ { } γ {2 5 2} γ {1 1 1} γ Table 2: Habit plane indices for martensite. With the exception of ɛ martensite, the quoted indices are approximate because the habit planes are in general irrational. Orientation Relationships The formation of martensite involves the coordinated movement of atoms. It follows that the austenite and martensite lattices will be intimately related. All martensitic transformations therefore lead to a reproducible orientation relationship between the parent and product lattices. It is frequently the case that a pair of corresponding close packed planes in the ferrite and austenite are parallel or nearly parallel, and it is usually the case that corresponding directions within these planes are roughly parallel (Fig. 2): {1 1 1} γ {0 1 1} α < > γ < > α Kurdjumov Sachs {1 1 1} γ {0 1 1} α Nishiyama Wasserman < > γ about 5.3 from < > α towards < > α {1 1 1} γ about 0.2 from{0 1 1} α Greninger Troiano < > γ about 2.7 from < > α towards < > α The body centred cubic lattice does not have a close packed plane but {0 1 1} α is the most densely packed plane. 3
4 Note that these have been stated approximately: the true relations are irrational, meaning that the indices of the parallel planes and directions cannot be expressed using rational numbers (the square root of 2 is not a rational number). Fig. 2: Stereographic representation of the Kurdjumov Sachs and Nishiyama Wasserman orientation relationships. The stereograms are both centred on (1 1 1) γ (0 1 1) α. It is seen that the NW orientation can be generated from KS by an appropriate small rotation (5.25 ) about [0 1 1] α. Only a few of the poles are marked to allow a comparison with the Bain orientation relationship. The neighbouring pairs of poles would superpose exactly for the Bain orientation. Athermal Nature of Transformation In the vast majority of cases, the extent of reaction is found to be virtually independent of time: 1 V α = exp{β(m S T)} where β (1) V α is the fraction of martensite and T is a temperature below M S. This is the Koistinen and Marburger equation; notice that time does not feature in this relation, so that the fraction of martensite depends only on the undercooling below the martensite start temperature. This athermal character is a consequence of very rapid nucleation and growth, so rapid that the time taken can in normal circumstances be neglected. Isothermal martensite is possible when nucleation is hindered, although the growth rate of individual plates of martensite can still be rapid. 4
5 Structure of the Interface Any process which contributes to the formation of martensite cannot rely on assistance from thermal activation. There must therefore exist a high level of continuity across the interface, which must be coherent and semi coherent. A stress free fully coherent interface is impossible for the γ α transformation since the lattice deformation BR is an invariant line strain. A semi coherent interface must be such that the interfacial dislocations can glide as the interface moves (climb is not permitted). It follows that the Burgers vectors of the interface dislocations must not lie in the interface plane unless the dislocations are screw in character. There is an additional condition for a semi coherent interface to be glissile. The line vectors of the interfacial dislocations must lie along an invariant line, i.e. a line which joins the parent and product crystals without any rotation or distortion. Why is that? If there is any distortion along the dislocation line, then other dislocations are needed to accommodate that misfit. It will then be necessary to have more than one set of non parallel dislocations in the interface. These non parallel dislocations can intersect to form jogs which render the interface sessile. It follows that for martensitic transformation to be possible, the deformation which changes the parent into the product must leave one or more lines invariant (unrotated, undistorted). A deformation which leaves one line invariant is called an invariant line strain. The Shape Deformation The passage of a slip dislocation through a crystal causes the formation of a step where the glide plane intersects the free surface (Fig. 3a,b). The passage of many such dislocations on parallel slip planes causes macroscopic shear (Fig. 3c,d). Slip causes a change in shape but not a change in the crystal structure, because the Burgers vectors of the dislocations are also lattice vectors. During martensitic transformation, the pattern in which the atoms in the parent crystal are arranged is deformed into that appropriate for martensite, there must be a corresponding change in the macroscopic shape of the crystal undergoing transformation. The dislocations responsible for the deformation are in the α /γ interface, with Burgers vectors such that in addition to deformation they also cause the change in crystal structure. The deformation is such that an initially flat surface becomes uniformly tilted about the line formed by the intersection of the interface plane with the free surface. Any scratch traversing the transformed 5
6 region is similarly deflected though the scratch remains connected at the α /γ interface. These observations, and others, confirm that the measured shape deformation is an invariant plane strain (Fig. 3e g) with a large shear component ( 0.22) and a small dilatational strain ( 0.03) directed normal to the habit plane. Fig. 3: (a, b) Step caused by the passage of a slip dislocation. (c, d) Many slip dislocations, causing a macroscopic shear. (e) An invariant plane strain with a uniaxial dilatation. (f) An invariant plane strain which is a simple shear. (g) An invariant plane strain which is the combined effect of a uniaxial dilatation and a simple shear. Bain Strain We now consider the nature of the strain necessary to transform the c.c.p. lattice of γ into the b.c.c. lattice of α. Such a strain was proposed by Bain in 1924 and hence is known 6
7 as the Bain Strain (Fig. 4). There is a compression along the z axis and a uniform expansion along the x and y axes. Fig. 4: The Bain strain (not all lattice points illustrated) The deformation describing the Bain Strain is given by B = ɛ ɛ ɛ 0 ɛ 0 = 2aα a γ a γ ɛ 0 = a α a γ a γ where a α and a γ are the lattice parameters of martensite and austenite respectively. The contraction is therefore along the [0 0 1] γ axis and a uniform expansion on the (0 0 1) γ plane. The Bain strain implies the following orientation relationship between the parent and product lattices: [0 0 1] fcc [0 0 1] bcc [1 1 0] fcc [1 0 0] bcc [1 1 0] fcc [0 1 0] bcc 7
8 but in fact, the experimentally observed orientation relationships are irrational, as discussed earlier. We shall deal with this inconsistency later. Temporarily neglecting the fact that the Bain orientation is inconsistent with experiments, we proceed to examine whether the Bain strain leaves at least one line invariant. After all, this is a necessary condition for martensitic transformation. In Fig. 5a,b, the austenite is represented as a sphere which, as a result of the Bain strain B, is deformed into an ellipsoid of revolution which represents the martensite. There are no lines which are left undistorted or unrotated by B. There are no lines in the (0 0 1) fcc plane which are undistorted. The lines wx and yz are undistorted but are rotated to the new positions w x and y z. Such rotated lines are not invariant. However, the combined effect of the Bain strain B and the rigid body rotation R is indeed an invariant line strain (ILS) because it brings yz and y z into coincidence (Fig. 5c). This is the reason why the observed irrational orientation relationship differs from that implied by the Bain strain. The rotation required to convert B into an ILS precisely corrects the Bain orientation into that which is observed experimentally. Fig. 5: (a) and (b) show the effect of the Bain strain on austenite, which when undeformed is represented as a sphere of diameter wx = yz in three dimensions. The strain transforms it to an ellipsoid of revolution. (c) shows the invariant line strain obtained by combining the Bain strain with a rigid body rotation through an angle θ. As can be seen from Fig. 5c, there is no rotation which can make B into an invariant plane strain since this would require two non parallel invariant lines. Thus, for the f cc bcc 8
9 transformation, austenite cannot be transformed into martensite by a homogeneous strain which is an IPS. And yet, the observed shape deformation leaves the habit plane undistorted and unrotated, i.e. it is an invariant plane strain. The phenomenological theory of martensite crystallography solves this remaining problem (Fig. 6). The Bain strain converts the structure of the parent phase into that of the product phase. When combined with an appropriate rigid body rotation, the net homogeneous lattice deformation RB is an invariant line strain (step a to c in Fig. 6). However, the observed shape deformation is an invariant plane strain P 1 (step a to b in Fig. 6), but this gives the wrong crystal structure. If a second homogeneous shear P 2 is combined with P 1 (step b to c), then the correct structure is obtained but the wrong shape since P 1 P 2 = RB These discrepancies are all resolved if the shape changing effect of P 2 is cancelled macroscopically by an inhomogeneous lattice invariant deformation, which may be slip or twinning as illustrated in Fig. 6. The theory explains all the observed features of the martensite crystallography. The orientation relationship is predicted by deducing the rotation needed to change the Bain strain into an invariant line strain. The habit plane does not have rational indices because the amount of lattice invariant deformation needed to recover the correct the macroscopic shape is not usually rational. The theory predicts a substructure in plates of martensite (either twins or slip steps) as is observed experimentally. The transformation goes to all the trouble of ensuring that the shape deformation is macroscopically an invariant plane strain because this reduces the strain energy when compared with the case where the shape deformation might be an invariant line strain. Thermodynamics of Martensitic Transformations Martensite is not represented on phase diagrams because the latter deal with equilibrium. Martensite deviates from equilibrium in two important ways: Martensite grows without diffusion, so it inherits the chemical composition of the parent austenite. In an equilibrium transformation the chemical elements partition into the parent and product phases in a manner which leads to a minimisation of free energy. Secondly, the shape deformation associated with martensitic transformation causes strains; the resulting strain energy has to be accounted for before the transformation can happen. 9
10 Fig. 6: The phenomenological theory of martensite crystallography These deviations can be represented on a free energy plot as illustrated in Fig. 7. The relationship with the phase diagram is illustrated in Fig. 8. Martensitic transformation is only possible below the T 0 temperature. 10
11 Fig. 7: The distance ac represents the free energy decrease when austenite of composition x decomposes into an equilibrium mixture of ferrite and austenite of compositions x αγ and x γα respectively. The distance ab is the smaller decrease in free energy when martensite forms without any composition change, taking into account the strain associated with the transformation. J mol 1 Strain energy 600 Twin interface energy 100 γ/α interface energy 1 Stored energy due to dislocations 20 Table 3: Typical energies associated with martensitic transformation. 11
12 Fig. 8: Schematic illustration of the origin of the T 0 curve on the phase diagram. The T 0 curve incorporates a strain energy term for the ferrite, illustrated on the diagram by raising the free energy curve for ferrite by an appropriate quantity. 12
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationLECTURE SUMMARY September 30th 2009
LECTURE SUMMARY September 30 th 2009 Key Lecture Topics Crystal Structures in Relation to Slip Systems Resolved Shear Stress Using a Stereographic Projection to Determine the Active Slip System Slip Planes
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationLecture 4: Thermodynamics of Diffusion: Spinodals
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 4: Thermodynamics of Diffusion: Spinodals Fick
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationChapter 8. Phase Diagrams
Phase Diagrams A phase in a material is a region that differ in its microstructure and or composition from another region Al Al 2 CuMg H 2 O(solid, ice) in H 2 O (liquid) 2 phases homogeneous in crystal
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationMaterial Deformations. Academic Resource Center
Material Deformations Academic Resource Center Agenda Origin of deformations Deformations & dislocations Dislocation motion Slip systems Stresses involved with deformation Deformation by twinning Origin
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationComposition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationDeformation of Single Crystals
Deformation of Single Crystals When a single crystal is deformed under a tensile stress, it is observed that plastic deformation occurs by slip on well defined parallel crystal planes. Sections of the
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationLecture 3: Models of Solutions
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP4, Thermodynamics and Phase Diagrams, H. K. D. H. Bhadeshia Lecture 3: Models of Solutions List of Symbols Symbol G M
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationSOLIDIFICATION. (a)formation of stable nuclei. Growth of a stable nucleus. (c) Grain structure
SOLIDIFICATION Most metals are melted and then cast into semifinished or finished shape. Solidification of a metal can be divided into the following steps: Formation of a stable nucleus Growth of a stable
More informationCrystal Symmetries METE 327 Physical Metallurgy Copyright 2008 Loren A. Jacobson 5/16/08
Crystal Symmetries Why should we be interested? Important physical properties depend on crystal structure Conductivity Magnetic properties Stiffness Strength These properties also often depend on crystal
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationUniversity of Cambridge, Materials Science & Metallurgy. Dilatometry
University of Cambridge, Materials Science & Metallurgy H. K. D. H. Bhadeshia Dilatometry The dilatometric method utilises either transformation strains or thermal strains; the basic data generated are
More informationIntroduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationHeat Treatment of Steels : Spheroidize annealing. Heat Treatment of Steels : Normalizing
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More information= 62 wt% Ni38 wt% Cu.
92 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationModule #17. Work/Strain Hardening. READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter
Module #17 Work/Strain Hardening READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter D. KuhlmannWilsdorf, Trans. AIME, v. 224 (1962) pp. 10471061 Work Hardening RECALL: During plastic deformation,
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationPhase transformation
Phase transformation Phase Transformation Topics o Basic principles relating to transformations o Kinetics of phase transformation: Nucleation and growth o Metastable and equilibrium state o Shape memory
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 5 Heat Treatment of Plain Carbon and Low
More information12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Crystal Geometry
12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Bibliography: Crystal Geometry Assigned Reading: [Poirier, 1985]Chapter 2, 4. General References: [Kelly and Groves, 1970] Chapter 1. [Hirth
More informationInvestigation of Titanium α Plates by EBSD Analysis
Investigation of Titanium α Plates by EBSD Analysis Master Thesis Arjen Kamp June 2007 Materials Science and Engineering Faculty 3mE Supervisors: Stefan van Bohemen Jilt Sietsma Roumen Petrov Investigation
More information3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?
ecture 1822: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationNPTEL: STRUCTURE OF MATERIALS Instructor: Anandh Subramaniam [Lecture1 to Lecture45] 1. Overview (C1) (Time: 49:06)
NPTEL: STRUCTURE OF MATERIALS Instructor: Anandh Subramaniam [Lecture1 to Lecture45] Lec Chapter 1. Overview (C1) (Time: 49:06) 2. Geometry of Crystals: Symmetry, Lattices (C2) (Time: 1:08:58) 3. (Time:
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationModule 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
More informationIntroduction to Materials Science, Chapter 11, Thermal Processing of Metal Alloys. Chapter 11 Thermal Processing of Metal Alloys
Chapter 11 Thermal Processing of Metal Alloys Designer Alloys: Utilize heat treatments to design optimum microstructures and mechanical properties (strength, ductility, hardness.) Strength in steels correlates
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationThe mechanical properties of metal affected by heat treatment are:
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
More informationPhase Equilibria & Phase Diagrams
Phase Equilibria & Phase Diagrams Week7 Material Sciences and Engineering MatE271 1 Motivation Phase diagram (Ch 9) Temperature Time Kinematics (Ch 10) New structure, concentration (mixing level) (at what
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationLMB Crystallography Course, 2013. Crystals, Symmetry and Space Groups Andrew Leslie
LMB Crystallography Course, 2013 Crystals, Symmetry and Space Groups Andrew Leslie Many of the slides were kindly provided by Erhard Hohenester (Imperial College), several other illustrations are from
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationPOSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL
1 POSSIBILITY OF INDIRECT HARDNESS TESTING OF DUPLEX STAINLESS STEEL István Mészáros Associate professor, Department of Materials Science and Engineering H1111 Budapest, Goldmann tér 3. Summary In this
More information9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure
913 9.8: 9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition
More informationMSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY
MSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of AlZnMgCu high strength alloy on isothermal
More informationTHE INVESTIGATION OF APPLICABILITY OF THE HOLLOMONJAFFE EQUATION ON TEMPERING THE HSLA STEEL
Available on line at Association of the Chemical Engineers AChE www.ache.org.rs/ciceq Chemical Industry & Chemical Engineering Quarterly 15 (3) 131 136 (2009) CI&CEQ ZORAN JANJUŠEVIĆ ZVONKO GULIŠIJA MARIJA
More informationPhase Transformations
Vysoká škola báňská Technická univerzita Ostrava Phase Transformations Didactic Text Vlastimil Vodárek Ostrava 2013 Review: Prof. Dr. Ing. Jaroslav Sojka Description: Phase Transformations Author: Vlastimil
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationME 612 Metal Forming and Theory of Plasticity. 1. Introduction
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In general, it is possible to evaluate metal forming operations
More informationCHAPTER 7: DISLOCATIONS AND STRENGTHENING
CHAPTER 7: DISLOCATIONS AND STRENGTHENING ISSUES TO ADDRESS... Why are dislocations observed primarily in metals and alloys? Mech 221  Notes 7 1 DISLOCATION MOTION Produces plastic deformation, in crystalline
More informationChapter Outline. Defects Introduction (I)
Crystals are like people, it is the defects in them which tend to make them interesting!  Colin Humphreys. Defects in Solids Chapter Outline 0D, Point defects vacancies interstitials impurities, weight
More informationLecture: 33. Solidification of Weld Metal
Lecture: 33 Solidification of Weld Metal This chapter presents common solidification mechanisms observed in weld metal and different modes of solidification. Influence of welding speed and heat input on
More informationDIFFUSION IN SOLIDS. Materials often heat treated to improve properties. Atomic diffusion occurs during heat treatment
DIFFUSION IN SOLIDS WHY STUDY DIFFUSION? Materials often heat treated to improve properties Atomic diffusion occurs during heat treatment Depending on situation higher or lower diffusion rates desired
More informationLecture 18 Strain Hardening And Recrystallization
138 Lecture 18 Strain Hardening And Recrystallization Strain Hardening We have previously seen that the flow stress (the stress necessary to produce a certain plastic strain rate) increases with increasing
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationWe shall first regard the dense sphere packing model. 1.1. Draw a two dimensional pattern of dense packing spheres. Identify the twodimensional
Set 3: Task 1 and 2 considers many of the examples that are given in the compendium. Crystal structures derived from sphere packing models may be used to describe metals (see task 2), ionical compounds
More informationGriffith theory of brittle fracture:
Griffith theory of brittle fracture: Observed fracture strength is always lower than theoretical cohesive strength. Griffith explained that the discrepancy is due to the inherent defects in brittle materials
More informationWelcome to the first lesson of third module which is on thinwalled pressure vessels part one which is on the application of stress and strain.
Strength of Materials Prof S. K. Bhattacharya Department of Civil Engineering Indian Institute of Technology, Kharagpur Lecture 15 Application of Stress by Strain Thinwalled Pressure Vessels  I Welcome
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
CHAPTER 8 DEFORMATION AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 8.1 To provide some perspective on the dimensions of atomic defects,
More informationDislocation theory. Subjects of interest
Chapter 5 Dislocation theory Subjects of interest Introduction/Objectives Observation of dislocation Burgers vector and the dislocation loop Dislocation in the FCC, HCP and BCC lattice Stress fields and
More informationBasic Concepts of Crystallography
Basic Concepts of Crystallography Language of Crystallography: Real Space Combination of local (point) symmetry elements, which include angular rotation, centersymmetric inversion, and reflection in mirror
More informationHW 8. G = a 3 G v. 6a 2. Problem a. To Find:
HW 8 Problem 10. a. To Find: (a) The expression for total free energy change for a cubic nucleus, critical cube edge length, a*, and G* (b) Compare G* for a cube with that for a sphere b. Given: Nucleus
More informationThe ClausiusClapeyron Equation:
Chapter 10 Solid Solutions and Phase Equilibrium What is a phase? Phase Diagram Basics A phase diagram represents what phases are present at a given pressure, temperature and composition. Virtual maps
More information1.3. DOT PRODUCT 19. 6. If θ is the angle (between 0 and π) between two nonzero vectors u and v,
1.3. DOT PRODUCT 19 1.3 Dot Product 1.3.1 Definitions and Properties The dot product is the first way to multiply two vectors. The definition we will give below may appear arbitrary. But it is not. It
More informationPhase. Gibbs Phase rule
Phase diagrams Phase A phase can be defined as a physically distinct and chemically homogeneous portion of a system that has a particular chemical composition and structure. Water in liquid or vapor state
More informationConcepts of Stress and Strain
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
More informationThe University of Western Ontario Department of Physics and Astronomy P2800 Fall 2008
P2800 Fall 2008 Questions (Total  20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
More informationMUKAVEMET KIRILMA HİPOTEZLERİ
1 MUKAVEMET KIRILMA HİPOTEZLERİ 17. Theories of failure or yield criteria (1) Maximum shearing stress theory (2) Octahedral shearing stress theory (3) Maximum normal stress theory for brittle materials.
More informationSolid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationEnergy of a Dislocation
Energy of a Dislocation The Line Tension T Broken and stretched bonds around the dislocation There is EXTRA energy associated with the Defect T = G 2 r 2 b J m G = Shear Modulus Total Extra Energy in the
More informationThis is an authordeposited version published in: http://sam.ensam.eu Handle ID:.http://hdl.handle.net/10985/10324
Science Arts & Métiers (SAM) is an open access repository that collects the work of Arts et Métiers ParisTech researchers and makes it freely available over the web where possible. This is an authordeposited
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationChapter 1 Introduction to Material science & Metallurgy
Chapter 1 Introduction to Material science & Metallurgy 1. Material Science & Metallurgy (21419) State the importance of study of materials science and briefly. Explain Engineering requirements of materials.
More informationx100 A o Percent cold work = %CW = A o A d Yield Stress Work Hardening Why? Cell Structures Pattern Formation
Work Hardening Dislocations interact with each other and assume configurations that restrict the movement of other dislocations. As the dislocation density increases there is an increase in the flow stress
More informationAnalysis of Stresses and Strains
Chapter 7 Analysis of Stresses and Strains 7.1 Introduction axial load = P / A torsional load in circular shaft = T / I p bending moment and shear force in beam = M y / I = V Q / I b in this chapter, we
More informationReflection and Refraction
Equipment Reflection and Refraction Acrylic block set, planeconcaveconvex universal mirror, cork board, cork board stand, pins, flashlight, protractor, ruler, mirror worksheet, rectangular block worksheet,
More informationHEAT UNIT 1.1 KINETIC THEORY OF GASES. 1.1.1 Introduction. 1.1.2 Postulates of Kinetic Theory of Gases
UNIT HEAT. KINETIC THEORY OF GASES.. Introduction Molecules have a diameter of the order of Å and the distance between them in a gas is 0 Å while the interaction distance in solids is very small. R. Clausius
More informationStereographic projections
Stereographic projections 1. Introduction The stereographic projection is a projection of points from the surface of a sphere on to its equatorial plane. The projection is defined as shown in Fig. 1. If
More informationEffect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel
International International Journal of ISSI, Journal Vol. of 12 ISSI, (2015), Vol.10 No.1, (2013), pp. 2832 No.1 Effect of Heat Treatment Process on the Fatigue Behavior of AISI 1060 Steel M. Mehdinia
More informationHeat Treating of Nonferrous Alloys
Metallogr. Microstruct. Anal. (2013) 2:190 195 DOI 10.1007/s1363201300748 TUTORIAL Heat Treating of Nonferrous Alloys Howard E. Boyer Ó American Society for Metals 1984 The reader should understand
More informationBINARY SYSTEMS. Definition of Composition: Atomic (molar) fraction. Atomic percent. Mass fraction. Mass percent (weight percent)
BINARY SYSTEMS Definition of Composition: Atomic (molar) fraction Atomic percent Mass fraction Mass percent (weight percent) na =, x i n = A i i i Weight percent mainly in industry! x at % A = x 100 A
More information3. APPLICATION OF PLASMA FOR HEAT TREATMENT
3. APPLICATION OF PLASMA FOR HEAT TREATMENT Classification of chapters: 3.1. Plasma 3.2. Physical metallurgical characteristics of quenched surface zone 3.2.1. Factors influencing achieved properties of
More informationUnit 6: EXTRUSION. Difficult to form metals like stainless steels, nickel based alloys and high temperature metals can also be extruded.
1 Unit 6: EXTRUSION Introduction: Extrusion is a metal working process in which cross section of metal is reduced by forcing the metal through a die orifice under high pressure. It is used to produce cylindrical
More informationCHAPTER 9 Part 1. = 5 wt% Sn95 wt% Pb C β. = 98 wt% Sn2 wt% Pb. = 77 wt% Ag23 wt% Cu. = 51 wt% Zn49 wt% Cu C γ. = 58 wt% Zn42 wt% Cu
CHAPTER 9 Part 1 9.5 This problem asks that we cite the phase or phases present for several alloys at specified temperatures. (a) For an alloy composed of 15 wt% Sn85 wt% Pb and at 100 C, from Figure
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationChapter 3: The Structure of Crystalline Solids
Sapphire: cryst. Al 2 O 3 Insulin : The Structure of Crystalline Solids Crystal: a solid composed of atoms, ions, or molecules arranged in a pattern that is repeated in three dimensions A material in which
More informationChapter 10: Phase Transformations
Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC γ (Austenite) Eutectoid transformation Fe 3 C (cementite) + α (ferrite) (BCC) How does the
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationModule 4 Design for Assembly IIT BOMBAY
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
More informationExperiment: Heat Treatment  Quenching & Tempering
Experiment: Heat Treatment  Quenching & Tempering Objectives 1) To investigate the conventional heat treatment procedures, such as quenching and annealing, used to alter the properties of steels. SAE
More information